Transcript of "Kokotov Et Al. 2009 Effect of Glass Dissolution on the Solution Deposition of ZnO Films and Its Exploitation for Deposition of Zn Silicates"
Published on Web 12/10/2009 Effect of Glass Dissolution on the Solution Deposition of ZnO Films and Its Exploitation for Deposition of Zn Silicates Michael Kokotov,† Shay Bar-Nachum,‡ Eran Edri,† and Gary Hodes*,† Department of Materials and Interfaces, Weizmann Institute of Science, RehoVot 76100, Israel, and The Jerusalem College of Engineering, Jerusalem 91035, Israel Received September 7, 2009; E-mail: firstname.lastname@example.org Abstract: ZnO is probably the most studied material deposited as ﬁlms by aqueous solution methods. Both neutral and alkaline solutions are commonly used, and deposition is often carried out in glass vessels. We show that for depositions carried out under alkaline conditions, slow dissolution of the glass by the solution often results in formation of zinc silicates together with the ZnO. While this silicate formation is most clearly seen after long deposition times (many hours), it can be detected already within 1 h, while often ZnO depositions proceed for substantially longer. We also describe conditions where the zinc silicate deposits without formation of ZnO providing a method of depositing such ﬁlms. Finally, we note that the glass of a reaction vessel also can affect deposition of CdSe, pointing to a more general role of this normally neglected parameter.Introduction effect of this attack in a CBD process (which are often carried ZnO is a readily available, nontoxic material that has many out at a fairly high pH) does not appear to have been consideredapplications, both actual and potential. As such, it is the subject to play an important role. In a continuation of our interest intoof very wide-ranging research. Of the numerous techniques used causes of irreproducibilities in CBD, we show in this Articleto prepare ZnO, solution methods have become very common, how the nature of the deposition vessel, speciﬁcally glass, candue to their simplicity and low temperatures. Chemical bath play a crucial role in the outcome of the ZnO deposition. Thedeposition (CBD)1 is the most common solution process used slowly dissolving SiO2 network introduces silicate ions in theto deposit ﬁlms of ZnO. It has been developed considerably ZnO deposition solution, resulting in the formation of Znsince it was ﬁrst described for this purpose by Call et al. in silicates on the ZnO ﬁlm.1980.2 (Liquid phase deposition and hydrothermal depositionare terms also used for essentially the same process, the latter While part of this Article is meant to demonstrate how onereferring more generally to solids whether as ﬁlms or as should be careful in the choice of the reaction vessel material,precipitates/powders.) While details of the mechanism may vary we also show how this knowledge can be exploited todepending on deposition, the generally accepted mechanism is deliberately deposit ﬁlms of Zn silicates, either on top of ZnOthrough dehydration of Zn-hydroxy complexes, which occur or instead of ZnO. Zn-rich Zn silicate-containing coatings arein the deposition solution, to form ZnO. The depositions are widely used for corrosion protection of steel.5 Because of itsnormally carried out at relatively high temperatures of 60-90 chemical stability and transparency in the ultraviolet and visible°C, which facilitate dissociation of the Zn complexes in the ranges, Zn silicate is also a commonly used material forsolution as well as dehydration. Despite its simplicity, CBD of phosphor preparation. Doped zinc silicate has high luminescenceZnO has a tendency to suffer from problems of reproducibility, efﬁciencies, and it is widely used in cathode ray tubes andand it is often extremely sensitive to deposition conditions.3 plasma display panels.6 It is also used in laser crystals,7 up-We previously showed how extremely low concentrations (<1 conversion luminescent materials,8 and other electroluminescentppm) of “impurities” (Fe, Mn) in the CBD solution can form devices.9 Zn silicate for such devices is usually produced byin situ nucleation centers on the substrate and allow ﬁlm growthunder conditions that would result in no deposit in the absence solid-state reaction methods employing high temperature coﬁringof the impurities.4 Most CBD processes are carried out in a glass vessel. Glass (5) (a) Thomas, A. Surf. Coat. Aust. 2009, 46, 10. (b) Hemmings, E. Surf.is known to be attacked by alkaline solutions. Despite this, the Coat. Aust. 2005, 42, 12. (c) Vkhristyuk, P. N. Fiz.-Khim. Mekh. Mater. 1983, 19, 26. † Weizmann Institute of Science. (6) Blasse, G.; Grabai, B. C. Luminescent Materials; Springer-Verlag: ‡ The Jerusalem College of Engineering. Berlin, 1994. (1) Hodes, G. Chemical Solution Deposition of Semiconductor Films; (7) Veremeichik, T. F.; Zharikov, E. V.; Subbotin, K. A. Cryst. Rep. 2003, Marcel Dekker: New York, Basel, 2003. 48, 974. Translated from: Kristallograﬁya 2003, 48, 1042. (2) Call, R. L.; Jaber, N. K.; Seshan, K.; Whyte Jr. Sol. Energy Mater. (8) Gerner, P.; Fuhrer, C.; Reinhard, C.; Gudel, H. U. J. Alloys Compd. 1980, 2, 373. 2004, 380, 39. (3) Govender, K.; Boyle, D. S.; Kenway, P. B.; O’Brien, P. J. Mater. (9) (a) Horng, R. H.; Wuu, D. S.; Yu, J. W. Mater. Chem. Phys. 1997, Chem. 2004, 14, 2575. 51, 11. (b) Ouyang, X.; Kitai, A. H.; Xiao, T. J. Appl. Phys. 1996, (4) Kokotov, M.; Biller, A.; Hodes, G. Chem. Mater. 2008, 20, 4542. 79, 3229.10.1021/ja907580u 2010 American Chemical Society J. AM. CHEM. SOC. 2010, 132, 309–314 9 309
ARTICLES Kokotov et al.of ZnO and SiO2 powders.10 Alternative methods include RFmagnetron sputtering,11 spray pyrolysis,12 sol-gel,13 polymerprecursor,14 and various hydrothermal methods.15 All of thesepublications (except refs 11 and 13b,c, which describe ﬁlmdeposition) describe the preparation of Zn silicate powders.Experimental Section Substrate Activation. In most experiments, the ﬁlms weredeposited on soda-lime glass microscope slides. (Other substrates,including various plastics and titanium, were also used with resultssimilar to those of glass.) The substrates were rinsed with Milliporedeionized water (DW) in an ultrasonic bath. For the surface activation, the substrates were placed in glass Figure 1. SEM cross-section (a) and plane view (b) of a ZnO ﬁlm depositedvials ﬁlled with 0.5 mM fresh KMnO4 solution.16 50 µL of at 92 °C for 40 min.n-butanol (as a reducing agent for the KMnO4) per 20 mL of thepermanganate solution was added. The vials were closed and placedin a water bath at 85 °C for 20-30 min. Permanganate-treatedsubstrates were extensively rinsed in DW (the vials containing thesamples were ﬁlled with DW, which was then poured out, and thiswas repeated for a total of 10 rinses) and then sonicated 5-10 minin DW in an ultrasonic bath. The extensive rinsing is important toprevent nucleation of ZnO in the bulk of the deposition solutionfrom Mn-containing particles detached from the treated substrate.The activation allows facile nucleation due to adsorption of Znspecies on the hydrated Mn oxide nuclei. In the absence ofactivation, little or no deposit forms.16 ZnO Film Deposition. Deposition solutions were prepared usingthe following aqueous stock solutions: 1.0 M ZnSO4 (for someexperiments, ZnAc2, ZnNO3, or ZnCl2 was used), 4.0 M ammoniumhydroxide, and 50% (by volume) monoethanolamine (2-aminoet-hanol). The ﬁnal deposition solution was prepared from the stock Figure 2. SEM images of ZnO ﬁlms deposited at 90 °C for 1 h and keptsolutions in 20 mL borosilicate glass vials (Wheaton liquid in the deposition solution at 75-80 °C for 5 days: (a,b) in a glass vial ((a)scintillation vials, part# 986541) or in polypropylene vials by dense ZnO ﬁlm, (b) open morphology ZnO ﬁlm from lower ammoniasequential addition to water of 1.0 mL of zinc salt, ∼1.5 mL of (complexant) concentration), (c) in a polypropylene vial.ammonia, and 2 mL of ethanolamine, giving the following ﬁnalconcentrations: 0.1 M Zn2+ (unless otherwise stated), 1.7 M (10% the substrate, the side chosen for characterization). The reactionv/v) ethanolamine, and ∼0.6 M NH3 (some results are shown for vial was closed and placed in a water bath at 75-95 °C. Theﬁlms deposited using a lower ammonia concentration ∼0.5 M; this deposition time varied from 0.5 to ∼350 h.will be designated as “lower ammonia concentration”). The amount More details of the permanganate activation of the substratesof water was chosen so that the total volume of each solution was and of the ZnO deposition have been described previously.1610 mL. The ﬁnal pH was typically 11.0-11.2. For some experi- Film Characterization. Films deposited on the bottom side ofments, crushed glass, either from the vials or from the soda-lime the substrates were ﬁrst visually inspected to monitor coatingglass microscope slides, was added to some vials. Immediately after uniformity on a macro scale. Scanning electron microscopy wasthe solution preparation, the substrate was placed in the solution carried out with a high resolution “Ultra 55” FEG Zeiss scanning(slightly inclined from vertical to prevent particles, which might electron microscope (SEM). Elemental analysis mapping was doneform in the solution from settling on the downward-facing side of by energy dispersive spectrometry (EDS) using an “OXFORD” detector in a SUPRA 55 VP FEG LEO SEM. Samples for cross-(10) (a) Schulman, J. H. J. Appl. Phys. 1946, 17, 902. (b) Brownlow, J. M.; section transition electron microscopy (TEM) were prepared using Chang, I. F. IEEE Trans. Electron DeVices 1983, ED-30, 479. (c) Guo, an FEI Helios dual beam focused ion beam (FIB) system. TEM Y.; Ohsato, H.; Kakimoto, K.-i. J. Eur. Ceram. Soc. 2006, 26, 1827. imaging and EDS analyses were done using a Philips CM120 TEM.(11) Minami, T.; Miyata, T.; Takata, S.; Fukuda, I. Jpn. J. Appl. Phys. 1991, 30, L117. X-ray diffraction (XRD) was carried out using a Rigaku RU300(12) Kang, Y. C.; Park, S. B. Mater. Res. Bull. 2000, 35, 1143. rotating anode X-ray diffractometer.(13) (a) Morimo, R.; Matae, K. Mater. Res. Bull. 1989, 24, 175. (b) Ji, Z.; Kun, L.; Yongliang, S.; Zhizhen, Y. J. Cryst. Growth 2003, 255, 353. Results (c) Copeland, T. S.; Lee, B. I.; Qi, J.; Elrod, A. K. J. Lumin. 2002, As shown in our previous work,16 uniform ZnO ﬁlms having 97, 168. (d) Lin, J.; Sanger, D. U.; Mennig, M.; Barner, K. Thin Solid Films 2000, 360, 39. typical morphology and crystal shapes shown in Figure 1 grow(14) Su, K.; Tilley, T. D.; Sailor, M. J. J. Am. Chem. Soc. 1996, 118, 3459. in about 40 min on substrates activated by permanganate. The(15) (a) Ahmadi, T. S.; Haase, M.; Weller, H. Mater. Res. Bull. 2000, 35, areal density of the ZnO crystals and the ﬁlm morphology (ZnO 1869. (b) Lu, S. W.; Copeland, T.; Lee, B. I.; Tong, W.; Wagner, B. K.; Park, W.; Zhang, F. J. Phys. Chem. Solids 2001, 62, 777. (c) crystal size and aspect ratio and directionality/texture) can be Yoon, C.; Shinboo, K. J. Mater. Res. 2001, 16, 1210. (d) Wang, H.; tailored by varying activation conditions, the complexant:Zn Ma, Y.; Yi, G.; Chen, D. Mater. Chem. Phys. 2003, 82, 414. (e) Wang, concentration ratio, and by choice of the anion of the zinc salt. H.; Zhuang, J.; Peng, Q.; Li, Y. J. Solid State Chem. 2005, 178, 2332. (f) Xiong, L.; Shi, J.; Gu, J.; Shen, W.; Dong, X.; Chen, H.; Zhang, More recently, we found that increasing the pH of the deposition L.; Gao, J.; Ruan, M. Small 2005, 1, 1044. (g) Li, Q. H.; Komarneni, solution results in ﬁlms with narrower ZnO crystals. S.; Roy, R. J. Mater. Sci. 1995, 30, 2358. (h) Wan, J.; Chen, X.; Wang, If, however, the deposition is continued for a much longer Z.; Mu, L.; Qian, Y. J. Cryst. Growth 2005, 280, 239. (i) Zeng, J. H.; time, the morphology of the ﬁlms changes signiﬁcantly (Figure Fu, H. L.; Lou, T. J.; Yu, Y.; Sun, Y. H.; Li, D. Y. Mater. Res. Bull. 2009, 44, 1106. 2a,b). The ﬁlms become very ﬁbrous, and individual rods appear(16) Kokotov, M.; Hodes, G. J. Mater. Chem. 2009, 19, 3847. to be composed of many ﬁbers. We initially thought that this310 J. AM. CHEM. SOC. 9 VOL. 132, NO. 1, 2010
Solution Deposition of ZnO Films ARTICLESFigure 3. SEM images of ZnO ﬁlms deposited at 90 °C (a) in a polypropylene vial - 3 h deposition; (b) in a glass vial - 1 h deposition; and (c) in a glassvial - 3 h deposition. The insets show lower magniﬁcation images. All three samples were placed together on one SEM sample holder, and all images weretaken using identical SEM operating parameters, including contrast and brightness. ﬁbrous ones, is found even under standard pH conditions (Figure 6b,c). Such dual morphology behavior of Zn silicate is described in the hydrothermal literature, showing a greater tendency for spherical morphology at lower pH or at lower ammonia concentration,15a,g,i the same as we ﬁnd for our ﬁlms. This dual morphology behavior of zinc silicate was also found in synthesis from organic solutions.18 SEM backscattered images of such ﬁlms clearly show thatFigure 4. SEM images of a ZnO ﬁlm deposited in a glass vial at 90 °C the overlayer on the ZnO has a lower average atomic numberfor 4 h and kept in the deposition solution at 80 °C for 4 h. (a) Plan view than that of the ZnO itself but higher that that of the glassand (b) cross-section view. substrate (Figure 7b together with the secondary electron image in Figure 7a). A cross-section EDS line scan through the ﬁlmﬁbrous structure was due to etching of the ZnO by the alkaline thickness (Figure 7c) shows that the overlayer consists of Si,solution after the Zn2+ concentration in the deposition bath Zn, and O in contrast to only Zn and O in the underlying ﬁlm.became low enough. However, under identical deposition It also shows that there is relatively more O and less Zn in theconditions, when plastic vials were used in place of glass ones, overlayer than in the ZnO underlayer. Cross-section TEMthis ﬁbrous morphology did not occur (Figure 2c).17 imaging of the ﬁlm (Figure 7d-h) reveals a nanogranular A change in surface appearance of the initially deposited structure (no crystal plane fringes were observed in thesmooth ZnO rods is already seen by SEM imaging after 1 h of nanograins) of the overlayer (Figure 7f) and the single crystaldeposition. Figure 3b shows the formation of white “spots” some nature of the ZnO rods (Figure 7g, which shows a smooth,nanometers in size on the top of a ZnO rod grown for 1 h in a featureless region of a ZnO crystal, and Figure 7h, a higherglass vial, suggesting formation of a different phase. The magniﬁcation image showing lattice fringes). The selected areadifference in contrast between the white spots and the darker electron diffraction patterns of the overlayer are very weak andZnO is due to electric potential difference between the spots broad but seem to match the powder pattern of ZnO. This(different charging of the spots as compared to that of the ZnO; indicates inclusions of some amount of ZnO nanocrystals inthe in-lens secondary electron detector used is particularly the apparently amorphous silicate phase. EDS/REM analysissensitive to charging effects). The growth of these “spots” of the overlayer gave an atomic % composition of: O ∼56%;continues until, after 3 h of growth, a continuous layer of this Si ∼12%; Zn ∼32%. In most cases, XRD of these ﬁlms doesphase is formed on the ZnO (Figure 3c). For ﬁlms grown under not reveal any additional phase besides the ZnO. However, inidentical conditions but in a plastic vial, no sign of this growth some samples, additional weak broad peaks and widening ofoccurs (Figure 3a). After 4 h, growth of a separate layer on the the ZnO (100) peak were observed (Figure 8). The broad peakssides of the ZnO rods, as well as on their tops, can be clearly can be best matched to a Na2Zn(Si2O6) phase.19 No correlationseen (Figure 4). The nature of the growth of this ﬁbrous layer was found between deposition condition or ﬁlm morphologydepends on the morphology of the ZnO rods. Under conditions and appearance of these peaks. Annealing of the ﬁlms atwhere open (loosely packed) ZnO rods form (in this case, by temperatures up to 500 °C (limited by the glass substrate) didusing a lower ammonia concentration), the layer grows on not affect the XRD pattern. Combining all of the above results,individual ZnO crystals (Figures 5a-c and 2b). For closer- together with the general observation from the literature thatpacked ZnO rods, this overlayer coalesces to form a dense the most usual phase for hydrothermally grown zinc silicate iscoating on the ZnO ﬁlm (Figures 5d-f and 2a). This ﬁbrous the willemite Zn2SiO4 phase, we consider that the most likelygrowth resembles the morphology of particles of Zn silicate composition for this overlayer is the willemite phase with somepowders obtained by hydrothermal methods (but at higher inclusions of nanocrystalline ZnO and maybe also sometemperature than our deposition conditions) as described in refs sodium-zinc silicate phase. (Na usually is not reliably detected15d,h,f,i. The maximum thickness of the overlayer is achieved by EDS due to its tendency to evaporate under the electronafter about 3 days, depending on the solution temperature. Amore spherical morphology of this overgrowth is obtained atslightly lower pH (10.8 instead of 11.0-11.2), as shown in (18) Lou, T. J.; Zeng, J. H.; Lou, X. D.; Fu, H. L.; Wang, Y. F.; Ma, R. L.; Tong, L. J.; Chen, Y. L. J. Colloid Interface Sci. 2007, 314,Figure 6a. On occasion, such a morphology, or a morphology 510.intermediate between that in Figure 6a and the more typical (19) There are at least dozens of alkali metal zinc silicate phases, each with a large number of peaks in the XRD pattern. Also, most well- deﬁned XRD patterns in the literature of zinc silicate compounds in(17) We note that most of the results shown in this Article were obtained general are obtained after high-temperature annealing. A positive using ZnSO4, but control experiments employing other zinc salts identiﬁcation of the measured XRD patterns in our case is therefore showed similar behavior, although with different rod diameters less than reliable. The exact composition and phase is not of great obtained depending on the anion of the Zn salt.16 relevance for this Article. J. AM. CHEM. SOC. 9 VOL. 132, NO. 1, 2010 311
ARTICLES Kokotov et al.Figure 5. SEM cross-section views of two series of ZnO ﬁlm depositions. (a-c) Films deposited from bath containing lower concentration of NH3, lessclosely packed and less aligned ZnO rods after 24, 140, and 270 h deposition respectively; (d-f) normal concentration of NH3, more closely packed andmore vertically aligned ZnO rods after 13, 63, and 120 h deposition, respectively. Note the magniﬁcation is not identical for the two series.Figure 6. SEM images of depositions showing (a) a repeatable spherical morphology at lower pH - acid added. Occasional spherical morphology obtainedusing (b) low ammonia concentration and (c) normal ammonia concentration.Figure 7. (a) Secondary electrons and (b) backscattered electron cross-section SEM images of dense ZnO ﬁlm with thick overlayer. (c) SEM EDS line scanmap across the ﬁlm cross-section. (d-h) Cross-section TEM images of a similar ﬁlm. (d) Upper parts of the ZnO rods covered with an overlayer (the darkgray and the black layers on top of the bright gray overlayer are metal ﬁlms deposited for FIB lamella cutting). (e) Zoom-in of a section of (d). (f) Zoom-inof the overlayer. (g) Zoom-in of the ZnO crystal. (h) High magniﬁcation lattice image of the ZnO crystal.beam.) If willemite and ZnO are indeed the two main phases, were added to the deposition solution in plastic vials. The ﬁlmthe semiquantitative TEM EDS results above are consistent with morphology in these cases was similar to that obtained usingan average overlayer atomic composition corresponding to a glass vials. This provides additional proof that formation of thecalculated volume ratio of 85% amorphous Zn2SiO4 and 15% Si-containing overlayer is due to dissolution of glass. A largernanocrystalline ZnO. amount of crushed glass or ﬁner glass pieces added to a As control experiments, pieces of broken glass (either from deposition solution result in faster formation of the crustsoda-lime glass microscope slides or borosilicate glass vials) overlayer, as expected. However, if sodium silicate is added to312 J. AM. CHEM. SOC. 9 VOL. 132, NO. 1, 2010
Solution Deposition of ZnO Films ARTICLES Figure 10. XRD pattern of an annealed (500 °C) ﬁlm deposited using aFigure 8. XRD pattern of ZnO ﬁlm covered by an overlayer as in Figure low concentration (25 mM) of zinc, other conditions as standard. The vertical5e. All sharp peaks belong to ZnO. The vertical lines show the database lines show the database pattern of the Zn2SiO4 (willemite, zinc silicate)pattern of the Na2Zn(Si2O6) phase (PDF#01-072-0741). phase (PDF#00-037-1485).the deposition solution at the start of deposition, a precipitate We can reasonably assume that the silicate overlayer forms whenforms immediately in the solution, and very little ﬁlm formation the Zn2+ concentration drops below the concentration at whichoccurs. Thus, slow release of silicate into the solution is ZnO can continue to grow and an equilibrium is establishednecessary for ﬁlm formation. between dissolution and growth of ZnO. If this assumption is It might be asked why the glass substrate itself does not true, then by starting with a low enough Zn2+ concentration (orsupply silicate ions to the deposition solution. ZnO deposition high enough complex:Zn ratio), we should be able to obtain aby CBD normally requires activation of the substrate to allow predominantly or even solely Zn silicate ﬁlm. Figure 9 showsZnO nucleation. While the glass substrates are activated (by SEM images of such ﬁlms using 25% of the original Znpermanganate treatment in this work), the vessel is not. Thus, concentration (25 mM instead of 100 mM), all other componentsthe ZnO layer, which forms only on the activated substrate, of the solution kept unchanged. Thin, apparently amorphous orprotects it against dissolution. We note that, for a long period of time, we were not aware very small crystal ﬁlms were observed on the glass substratesof the silicate formation and thought that it was ZnO possessing using ZnCl2 (or ZnSO4) (Figure 9a,b). Extremely stronga novel morphology. It was only after carrying out cross-section adhesion of the ﬁlm to the substrate is indicated by thebackscattered SEM (of particularly long depositions) that we continuous crack lines, from the sample fracture, across therealized there was a difference in composition between the ZnO interface (Figure 9b). No XRD pattern was found from theseand what we eventually realized was silicate and that some as-deposited ﬁlms. After being annealed at 500 °C for 1 h insilicate already started to form even after short depositions, air, two types of crystals could be seen in the SEM images:although this was not readily visible in its early stages in SEM large ill-deﬁned crystals inside the ﬁlm (Figure 9d,f) and smallerimaging. Also, as noted above, the silicate would not be seen faceted crystals embedded into the ﬁlm surface (Figure 9e) (noby XRD because no (or virtually no) XRD pattern is seen, even atomic weight contrast is seen by backscattered imaging in eitherafter thick layers of silicate had formed. annealed or as-deposited ﬁlms (Figure 9c,f)). Longer annealing Using our deposition conditions, ZnO ﬁlm growth is a fast at the same temperature did not change this picture. Weak XRDprocess; it takes about 40 min until the ZnO ﬁlm reaches its peaks indicating the presence of Zn2SiO4 (willemite zinc silicate)maximal thickness (this is faster than most other ZnO baths). appeared after annealing (Figure 10).19Figure 9. SEM secondary electron (a,b,d,e) and backscattered (c,f) images of a silicate ﬁlm deposited using a low concentration of zinc (25 mM ZnCl2).As deposited (a,b,c), annealed (d,e,f). Part (e) shows a zoomed-in region of the surface. J. AM. CHEM. SOC. 9 VOL. 132, NO. 1, 2010 313
ARTICLES Kokotov et al. Finally, in view of our interest in nanoporous solar cells, we containing nitrilotriacetic acid as a complexing agent,21 proceedsfabricated ZnO/CdSe/CuSCN solar cells using CBD ZnO on much faster in a borosilicate vial than in a plastic one.SnO2-conducting glass.20 Three cells were made using ZnO Furthermore, if some pieces of soda-lime glass are introduceddeposited in glass vials and three cells using ZnO deposited into such a bath, a substantial amount of Si is incorporated intounder identical conditions but in plastic vials. In all cases, the the resulting ﬁlms. The possibility of formation of silicates hascells made in plastic vials gave open circuit voltages that were to be taken into account because they can dramatically altersigniﬁcantly higher (by g70 mV) than the control cells made chemical, structural, and electronic properties of the depositedusing ZnO deposited in glass vials (the other cell parameters ﬁlms. In preliminary experiments, the open circuit voltage ofdid not vary in any systematic way between the two types of CdSe-sensitized ZnO nanoporous solar cells is increasedZnO). While preliminary, these experiments emphasize the considerably if the CBD ZnO is grown in a plastic vial asimportance of the nature of the reaction vessel in ZnO compared to a glass one.deposition. We also present preliminary results that exploit this phenom-Conclusions enon to deliberately grow Zn silicate ﬁlms, an important Chemical bath deposition (CBD) of ZnO from alkaline compound for luminescence and anticorrosion applications. Insolution in a glass reaction vessel gives initially ZnO, but an this case, a low starting concentration of Zn in the depositionalkali metal Zn silicate phase forms as an overlayer on the ZnO solution prevents growth of ZnO, and only the silicate is formedas the Zn concentration in the bath decreases with time and as a very adherent ﬁlm on glass substrates. Silicates of Zn cannotthis overlayer becomes thicker with increasing growth time. This be grown simply by adding alkali metal silicate solution to thephase forms due to slow etching of the glass vessel (both deposition bath as immediate precipitation occurs; the slowborosilicate and soda-lime glass behave similarly) at the pH of release of the soluble silicate is essential for this deposition.the solution (ca. 11). This etching gradually releases silicate The source of the Si can be either the glass vessel itself orions to the solution, which react to give the silicate. Using plastic deliberately-added glass.reaction vessels, only ZnO is formed regardless of the depositiontime. While etching of glass in strongly alkaline solution is well- Acknowledgment. This work was supported by the US-Israelknown, these results show that even under relatively mild Binational Science Foundation and the Alternative Energy Researchalkaline condition, glass etching occurs and, more importantly, Initiative (AERI). We thank Dr. Yishay Feldman for help with XRDcan completely change the nature of the deposit. Recently, we analysis, Dr. Palle von Huth for help with FIB sample cross-have noted that the inﬂuence of glass is not limited to ZnO sectioning, and Dr. Ronit Popovitz-Biro for help with TEM imaging.depositions but that it is more general. Ion-by-ion deposition The electron microscopy studies were conducted at the Irving andof CdSe, carried out under alkaline conditions from solutions Cherna Moskowitz Center for Nano and Bio-Nano Imaging at the Weizmann Institute of Science. We acknowledge the Harold(20) Levy-Clement, C.; Tena-Zaera, R.; Ryan, M. A.; Katty, A.; Hodes, Perlman family’s historic generosity. G. AdV. Mater. 2005, 17, 1512.(21) Gorer, S.; Hodes, G. J. Phys. Chem. 1994, 98, 5338. JA907580U314 J. AM. CHEM. SOC. 9 VOL. 132, NO. 1, 2010